p o l y ~ Phomeht, miary 1 (1981) 69--80
PHOTO-OXIDATION OF EPOXY RESINS CURED BY NON-AROMATIC AMINES
V. B m T~NGER, C. BOUCHARD, P. CLAVEmOLLE and J. VERDU
Depattemenz Materiaux, ENSAM, 151 Bd de l'H~pital, 75640, Paris 13, France
The photo-oxidation of epoxy resins based on bisphenol A and cured by non-aromatic amines: diethylene triamine, aminoethyl piperazine and isophorone diamine results in carbonyl and amide formation, decrease of glass transition temperature, and the appearance of a new endotherm at 70-80C in the DSC traces. The carbonyl and, essentially the amide yield depend strongly on the hardener structure and concentration. The mechanisms of formation of these groups are discussed.
Although epoxy based composites are often used in conditions involving direct exposure to sunlight, the photochemical ageing of these materials has received little attention in comparison to thermal or hydrolytic ageing. 1 Conventional methods are used to characterise the change in optical (yellowing), electrical2 or mechanical2"3 properties during natural or artificial ageing. The changes in the macromolecular skeleton due to photo-oxidation, can lead to surface stresses, possibly responsible for microcrazing as observed by electron microscopy.4 The simultaneous use of methods such as FTIR spectroscopy, ESCA thermogravimetry, laser pyrolysis and dynamic mechanical measurements for the study of natural and artificial ageing of an epoxy novolacbased composite leads to the following observations: s'6 (1) The thermal stability decreases during UV exposure. Here the presence of water has a strong accelerating effect. (2) The ageing results in a decrease in the glass transition 69Polymer Photochemistry 0 1 4 4 - 2 8 8 0 / 8 1 / 0 0 0 1 - 0 0 6 9 / $ 2 - 5 0 ( ~ ) A p p l i e dEngland, 1981 Printed in N o r t h e r n Ireland Science Publishers Ltd,
V. B~.l ~ .~NGER, C. BOUCHARD, P. CLAVEIROLLE, J. VERDU
temperature and erosion of superficial layers. (3) Therrnal oxidation during the cure treatments has a significant photosensitising effect, the photostability is improved by the use of antioxidants. (4) Resins based on bisphenol A are more stable than epoxy novolacs. In the case of diglycidyl ether of bisphenol A (DGEBA) systems, some mechanistic data on photodegradation and photooxidation can be derived from the results obtained with phenoxy resins, which contain the bisphenol and glyceryl structures: The aim of our work is to study the photo-oxidation kinetics and mechanisms of epoxy resins and, if possible, to establish the structure-properties relationship in this area. The present paper is devoted to the study of non-aromatic amine hardeners including diethylene triamine, aminoethyl piperazine and isophorone diamine in DGEBA systems.
The polymers were prepared from a diglycidyl ether of bisphenol A (DGEBA) which had an epoxy index of 5"30M/kg. The samples were denoted by a code consisting of the abbreviation used for the hardener: DETA for diethylene triamine, AEP for aminoethyl piperazine and IPD for isophorone diamine. All products were Ciba Geigy industrial grades. Two sets of samples were studied. In the first, the amine concentration was close to the stoiehiometric value; in the second, we studied the influence of hardener concentration for the D G E B A - D E T A system. The code indicates the DETA concentration in per cent of the stoichiometric value. Films, 24 ~m thick, were cast on a clean mercury surface from a solution of the two components in benzene (Prolabo analytical grade). After 2 h at 120C, the solvent was evaporated off (controlled at 675 cm-1 in the IR spectrum) and a hard transparent film was obtained. For IR quantitative measurements (Perkin-Elmer 580), we used the peak at 1885 cm -1 as the internal standard. Absorbance at 1885 cm -1 per thickness u n i t = 2 6 + 6 c m -1. We verified that the extinction coefficient of this band is independent of hardener structure and ageing time. The extinction coefficient of hydroxyl groups has been calculated from the data obtained with the DETA 50 sample, assuming a 100% conversion of the amine-epoxide reaction and taking into account the contribution of D G E B A (calculated value: [OH]=0.34M/kg). The result, eoH= 44 kg M -~ cm -~, agrees reasonably well with the literature data and allows an estimation of the conversion factor for the other samples. The initial characteristics of the films are summarised in Table 1. DSC measurements (for three samples) were taken before and after exposure. For photo-oxidation studies, we used a reactor equipped with a fluorescent
PHOTO-OXIDATION OF EPOXY RESINS CURED BY NON-AROMATIC AMINES TABLE 1 INITIAL DATA Nit hardener (M/kg) 0 5.42 5-42 5.16 5.16 5.30 5-30 2.65 3.98 5"30 6.63 Thermal treatment (h) at 120"C 0 2 5 2 5 2 5 8 2 2 2
Sample DGEBA IPD IPD (T) AEP A E P (T) DETA D E T A (T) DETA DETA DETA DETA 50 75 100 125
Hardener (M/kg) 0 1.36 1.36 1.29 1.29 1.06 1.06 0.53 0.80 1-06 1.33
AOH -12.9 14.5 7.7 9.0 9.4 10.4 5.1 7-3 9"4 9"9
Aco 0 0.17 0.36 0.53 0.50 0.18 0-27 0.25 0.23 0"18 0-31
Ta ACON/~ (K) 0 0 0 0 0.7 0 0-9 0 0 0 0 -405 -383 -373 ------
Absorbance of peak i Note: A i Absorbance of 1885 cm -1 peak
lamp: Osram L 20 W 70 emitting between 300 and 450 nm. The overall light intensity at the sample level is 24x 1014 photons cm -2 s-1 (ferrioxalate actinometry). In the first experiment, the samples were exposed for 189 h at 27C, we calculated the mean rates: rco and rcoN(, and determined graphically the initial rates of carbonyl rico and amide ricoN~ formation from the kinetic curves of the 1725 and 1660 cm -1 peak growth. In the second experiment, the samples were exposed for 70 h at 60C and we only determined initial rates. Despite the relative inaccuracy of these last values, the activation energies were estimated.
1. Photo-oxidation of D G E B A at 27C (capillary trim on CaFz plate) We observed an essentially carbonyl formation (maximum absorbance at 1735 cm-1). A small peak appears also at 1670 cm -1, which could be attributed to conjugated oxidation products of the bisphenol moiety. The hydroxyl absorbance increases only after a long induction period (500 h). 2. Influence of the hardener structure (27C exposure) We observed changes in the IR spectrum in three distinct regions: the hydroxyl region (3400cm-1), the carbonyl region (1725-1735 cm-1) and the amide
v. BI=IJ.RNGER, C. BOUCHARD, P. CLAVEIROI ] ~.. J. VERDU1, 5' [ko
h 200DETA; D, D E T A
A (carbonyl) versus exposure time at 27C: O, IPD; Q, IPD (T); i (T); &,, AEP; A, A E P (T)
A (amide) venus exposure time at 27C, same symbols as in Fig. 1.
PHOTO-OXIDATION OF EPOXY RESINS C U R E D BY NON-AROMATIC AMINES
region (1650-1660 cm-1). The kinetic curves of carbonyl and amide growth are given in Figs 1 and 2, respectively. The mean rates of normalised absorbance variation are given in Table 2. The behaviour of the three systems can be summarised as follows: (1) IPD has the higher carbonyl yield and the lower amide yield (2) AEP shows exactly the opposite behaviour, and D E T A is intermediary. TABLE 2MEAN RATES OF CARBONYL AND AMIDE GROWTH. I N F L ~ C ~ TREATMENT OF HARDENER STRUCTURE AND THERMAL
[~ Ca,do(M/kg) 6-80 6.80 9.54 9.54 15.48 15.48
r~o*( x l 0 - a h -1 ) 3.7 5.3 2.1 3.7 1.0 1.6
r~o~C.( x 1 0 - 3 h -1 ) 3.2 4.2 7-4 8.5 16.4 16.4 Pcor~( b 0.47 0-62 0.77 0.89 1.06 1.06
r, (K) 388 -363 -371 --
SamplesIPD I P D (T) DETA D E T A (T) AEP A E P (T) Note:
(Mlkg) 7-56 -5.51 -4-51 --
1 ~ 10 3 h -1, w h e r e A i = a b s o r b a n c e of p e a k j. a ri = A1885cm-1 At TCON~ b PCON~ [ a C H 2 ] c A f t e r 189 h e x p o s u r e .
The amide groups were derived from an oxidative attack of the methylene groups:/hr.02 _
O Assuming a 100% conversion of the amine-epoxide reaction, we have calculated the initial a methylene concentration and the amide yield during photooxidation: Pco~'~ =rate of amide growth per initial a methylenic unit. The higher yield is found in A E P samples, the lower in IPD samples, D E T A being intermediary (Table 2). DSC data shows that there is a slight decrease in Ta but, essentially, it shows the appearance of a new endothermic peak near the 70C point (Fig. 3 and Table 2).
3. Influence of thermal treatment Thermal treatment at 120C in air results in a thermo-oxidation: carbonyl groups appear in IPD and D E T A samples, whereas amide groups appear in
v. BTRT.T.I~.NOER, C. BOUC~ARD, P. ~'V]EII~OT! .~ J. VERDU
t 100Fig. 3.
DSC curves for DETA 100 before (above) and after (below) U V exposure. V, glass transition and V, new endotherm.
olFig. 4. A (carbonyl) versus exposure time at 27C for the DETA systems. O, D E T A 50; 1"7, DETA 75; O, D E T A 100; &, DETA 125.
PHOTO-OXIDATION OF EPOXY RESINS CURED BY NON-AROMATIC AMINES
A (amide) versus exposure time at 27C for the DETA systems, same symbols as in Fig. 3.
s a m p l e s ( T a b l e 1). T h i s t h e r m a l o x i d a t i o n h a s a s l i g h t b u t a g e i n g ( T a b l e 2)
noticeable sensitising effect on subsequent photochemical
4. Influence of hardener concentration ( D E T A )A t 2 7 C , t h e m e a n r a t e o f c a r b o n y l g r o w